2 / Aluminum Alloy Castings: Properties, Processes, and Applicationscasting process. Continuing technological improvements in alloy, An ability to produce near-net-shape parts with dimensionalcasting, and recycling technology have improved the competitive- accuracy, controlled surface ﬁnish, complex geometries includingness and enhanced the growth of aluminum castings markets. internal passages, and properties consistent with speciﬁed engi- neering requirements represents signiﬁcant manufacturing advan- tages (Fig. 1.1, 1.2):1.3 Advantages and Limitations of Aluminum Castings • In many cases, multicomponent welded or joined assemblies can be replaced with a single cast part. Aluminum castings are produced in a range of alloys demon- • Machining requirements are reduced.strating wide versatility in the characteristics than can be achieved. • Aluminum castings display controlled variations in as-castMore than 100 compositions are registered with the Aluminum ﬁnish.Association, and more than 300 alloys are in international use. • Contrasts between as-cast and machined ﬁnishes can be high-Properties displayed by these alloys, without considering the ex- lighted to create pleasing cosmetic effects.panded capabilities of metal-matrix and other composite structures, • Capital requirements are typically less than for wrought prod-include: ucts. • Tooling can range from simple patterns to complex tool steel dies depending on product requirements and production vol-Tensile strength, ksi (MPa) 10–72 (70–505) ume.Yield strength, ksi (MPa) 3–65 (20–455)Elongation, % <1–30 • Metallurgically or mechanically bonded bimetal parts can beHardness, HB 30–150 routinely cast.Electrical conductivity, %IACS 18–60Thermal conductivity, Btu · in./h · ft2 · °F at 77 °F 660–1155 (85–175) • Aluminum parts are routinely cast by every known process, (W/m · K at 25 °C) offering a broad range of volume, productivity, quality, mecha-Fatigue limit, ksi (MPa) 8–21 (55–145)Coefficient of linear thermal expansion 9.8–13.7 ϫ 10–6/°F nization, and specialized capabilities. at 68–212 °F (20–100 °C) (17.6–24.7) ϫ 10–6/°C) • Most aluminum casting alloys display solidiﬁcation character-Shear strength, ksi (MPa) 6–46 (42–325)Modulus of elasticity, 106 psi (GPa) 9.5–11.2 (65–80) istics compatible with foundry requirements for the productionSpeciﬁc gravity 2.57–2.95 of quality parts.Fig. 1.1 Casting applications include innovative and complex designs serving the needs of diverse industries. (a) Aircraft stabilizer. (b) Golf irons. (c) Crankcase for small engine. (d) Cross member for a minivan. (e) Cellular phone casing. Source: Ref 1
Chapter 1: Introduction / 3• Many aluminum casting alloys display excellent ﬂuidity for the incentives to reduce fuel consumption while preserving product casting thin sections and ﬁne detail. performance and cost objectives.• Aluminum casting alloys melt at relatively low temperatures. The most cost-effective means of addressing these challenges• Aluminum casting processes can be highly automated. has been the substitution of lightweight materials in existing and projected automotive designs. The U.S. automotive industry in Many limitations do apply. Very thin sections may not be castable. collaboration with suppliers and the U.S. Department of EnergyThere are practical limitations in size for speciﬁc casting processes. formed coalitions, including USAMP, which focused on materialsThe solidiﬁcation behavior of some alloys precludes casting in characterization, and USCAR, which focused on materials devel-difficult engineered conﬁgurations or in speciﬁc casting processes. opment and process capabilities. Their objective has been to fa-The casting process is simpler and less capital intense than pro- cilitate the transition to lighter-weight materials and more fuel-cesses for producing forgings, extrusions, and rolled products. How- efficient performance without sacriﬁce in safety and with minimalever, solidiﬁcation in complex geometrical shapes, as with other impact on costfabrication options, can result in surface discontinuities and inter- The emphasis placed on improved efficiency in energy-nal microstructure features with varying degrees of quality that consuming applications has resulted in a steady increase in theaffect properties and performance. production and use of aluminum castings. The recent pattern of Aluminum alloy castings can display the tensile properties of growth in aluminum casting shipments in the United States, in-most forgings, extrusions, and rolled plate. Because wrought prod- cluding projections through the year 2005 is (Ref 2):ucts are normally characterized by ﬁnely recrystallized grain struc-tures with speciﬁc anisotropy and highly textured microstructural Casting shipments in the United Statesfeatures, ductility in longitudinal directions is typically greater than Year 106 lb 106 kgin castings that contain coarser grain structures. Conversely, thetypically uniaxial grain structure and absence of anisotropy in cast 1994 2880 1306 1995 2990 1356structures do not present design engineers with the challenges 1996 3260 1479associated with transverse property limitations. 1997 3380 1533 1998 3490 1583 1999 3550 1610 2000 3640 1651 2001 3800 17241.4 Major Trends Inﬂuencing 2202 4100 1860 2003 4500 2041 Increased Use of Aluminum Castings 2004 4900 2223 2005 5160 23411.4.1 Technology The importance of improved energy efficiency in recent decadesreﬂects the effects of increased gasoline and oil costs to the con- Cast aluminum has been used or demonstrated successfully for many decades in power-train applications including engine blocks,sumer and graduated government-mandated fuel-efficiency stan-dards for automobile and truck manufacturers. Environmental con- cylinder heads, pistons, transmission cases, and oil pans. In the ﬁrst wave of light-weighting, aluminum was extensively adopted forcerns, global competitiveness, and raw-material concerns reinforce these parts. For maximum impact on fuel efficiency, this expansion in the role of cast aluminum necessitated substitutions in more critical structural parts requiring the qualiﬁcation of new compo- nent designs, materials, and production methods. These applica- tions include traditionally cast iron, malleable iron, nodular iron and steel cross members, suspension and control arms, brackets, brake valves, rotors, and calipers. The commercialization of alu- minum-intense automobile designs can result in 20 lb less engine emissions over the life of an automobile for each pound of iron or steel replaced by lower-density aluminum with correspondingly signiﬁcant reductions in fuel consumption (Ref 3). New aluminum- intensive automotive construction concepts include cast ﬁttings or nodes for extruded stringers in monocoque assemblies and the development of energy-absorbing thin-wall cast space frames. Fig- ures 1.3 through 1.6 summarize the results of a study performed for the Aluminum Association showing the growth in cast alumi- num as well as total aluminum products in North American light vehicle production. The most signiﬁcant barrier to the acceptance of cast alumi- num in these and many other structural applications has been itsFig. 1.2 One-piece cast missile tail cone. A cost-effective and reliable reputation for variability. Overcoming this barrier required the alternative to what had been a multicomponent assembly demonstration of integrity and reliability derived from the evolu-
4 / Aluminum Alloy Castings: Properties, Processes, and Applications tion of manufacturing processes and effective process controls. To be economic, casting results must be consistent and predictable without reliance on extensive inspection and nondestructive evalu- ation. Each step in these developments has been the product of close collaboration between aluminum casting suppliers and the auto- motive industry. Not only are speciﬁc engineering criteria to be met for each new component, process designs and controls must reli- ably demonstrate capability and consistent product quality in theFig. 1.3 North American light vehicle change in aluminum content, 1991 high volumes that are required. New casting processes, alloys, to 2002 composite compositions, thermal treatments, process control meth- odologies, and the sensors and controls they require have contrib- uted to an accelerated evolution of technologies that has been facilitated by research and development programs, many of which were sponsored by USCAR and USAMP in cooperation with na- tional laboratories, colleges, and universities and with supplier industries. Aluminum castings will play an important future role when in- evitable electric, hybrid, or fuel-cell technologies are developed to combine materials, design, and construction methods for maximum efficiency. Technological progress achieved in automotive programs affects all phases of aluminum foundry operations and all casting appli- cations. Technology is also being broadly advanced by the activi- ties of the U.S. Department of Energy that has identiﬁed metal casting as one of nine important “Industries of the Future.” Beneﬁts have been the development of a technology roadmap (Ref 4) that includes many of the challenges and technical barriers facing the aluminum castings industry and the funding of research and de- velopment programs in casting, aluminum, sensors, automation, and industrial materials of the future to meet or overcome them.Fig. 1.4 North American light vehicle change in aluminum content, 1991 The product of these efforts has been greater versatility and to 2002. (a) Passenger cars. (b) Trucks improved capability in consistently and economically meeting even the most severe engineering challenges in automotive and other industries. Understanding the material and process changes that areAluminum product form 1999 lb/vehicle Percent of total 2002 lb/vehicle Percent of total Percent change 1999 vs 2002Die castings 95.76 38.2% 101.42 37.1% ϩ5.9% or 5.66 lbPermanent mold castings 92.43 36.9% 100.58 36.8% ϩ8.8% or 8.15 lbFlat rolled products 27.24 10.9% 29.39 10.7% ϩ7.9% or 2.15 lbExtruded and drawn products 16.83 6.7% 18.49 6.8% ϩ9.9% or 1.66 lbForgings and impacts 6.34 2.5% 6.10 2.2% –3.8% or –0.24 lbSand, lost foam, squeeze, and semisolid castings 11.94 4.8% 17.52 6.4% ϩ46.7% or 5.58 lbTotal 250.54 100% 273.50 100% ϩ9.2% or 22.96 lbFig. 1.5 North American light vehicle change in aluminum content by product form and metal source, 1999 to 2002
Chapter 1: Introduction / 5taking place to further increase the comfort of design engineers in with competing materials, the advantage of aluminum in life-cyclethe use of aluminum castings is essential for deﬁning material analysis can be signiﬁcant.advantages for any new application. 1.5 Selecting the Right1.4.2 Recycling Aluminum Alloy and Casting Process Recycling and its impact in life-cycle studies are increasinglyimportant considerations in materials selection (Ref 5). The manner The succeeding chapters review the substantial portfolio of alu-in which energy efficiency can be directly and indirectly affected minum casting alloys available; Chapter 2 illustrates the charac-is important, but so are environmental and competitive consider- teristics that have made certain alloys the ﬁrst choice for speciﬁcations. While the production of aluminum is energy-intensive, it applications. Chapters 3 through 7 focus on the process and thermalcan be efficiently recovered from scrap at 5% of the energy required treatment variables that inﬂuence the metallurgical structure offor reduction. Corrosion resistance preserves metal value, and new aluminum alloys and, in turn, how the combination of processtechnologies are being developed for the segregation of scrap variables and metallurgical structure inﬂuence their properties andstreams by alloy and product form for essentially closed-loop re- performance. Finally, Chapter 8 provides a broad range of physicalcycling. and mechanical property data, a substantial amount of which has Virtually all aluminum forms classiﬁed as old scrap (end of never been published before, certainly not all in a single resource.cycle) and new scrap (turnings, borings, gates and risers, rejec- This wide range of information contained herein is provided astions) are recyclable. With appropriate recycling processes, recov- a reference for aluminum alloy casting producers, heat treaters,eries typically exceed 90%. designers, and users with the intent of aiding them in the selection Many casting compositions are compatible with the alloy con- of the right alloy, temper, and processing needed to achieve thetent of even mixed scrap. The cost of ingot produced from scrap performance required of cast components. The authors believe itis typically less than that of primary metal. As a consequence, most is clear that, as suggested above, aluminum casting alloys providealuminum alloy castings are produced from recycled metal. a broad range of capabilities including—when appropriate, process- The use of aluminum in energy-consuming applications pro- optimization and quality-control procedures are applied—compo-vides efficiencies with calculable beneﬁts for prolonging product nents suitable for challenging applications where soundness,life, conserving raw materials, reducing energy consumption in strength, and toughness are critical. The authors hope it will also bemanufacturing and service, reducing levels of environmental pol- clear that there are great advantages for designers and castinglution and the costs of environmental control, and lowering ma- suppliers working closely with their customers on the selection ofterial cost through recycling. When factored into cost comparisons alloys, tempers, and casting processes capable of meeting manu-Fig. 1.6 North American light vehicle change in aluminum content, 1973 to 2002
6 / Aluminum Alloy Castings: Properties, Processes, and Applicationsfacturing objectives, component performance criteria, and eco- • Aluminum, the Magic Metal, National Geographic, Aug 1978nomic targets. • Aluminum Permanent Mold Handbook, American Foundry So- This reference volume is not intended as a guide to producing ciety, 2001, 216 pagesaluminum alloy castings; for example, it does not cover the details • R.J. Anderson and H. Carey, The Metallurgy of Aluminium andof how to design and build molds, inject the molten alloys, and Aluminium Alloys, Baird and Company, 1925sequence the ﬁnishing process. For more information on such mat- • L. Arnberg, L. Bäckerud, and A. Dahle, Castability of Alumi-ters, the reader is referred to the excellent aluminum casting in- num Foundry Alloys, AFS Research Report, American Found-dustry publications of the American Foundry Society and similar rymen’s Society, 1999, 111 pagesorganizations (Ref 1, 6–9) plus those of the Aluminum Association • C.C. Carr, Alcoa, An American Enterprise, Rinehart and Com-(Ref 10–12). For those interested in a broader overview of the pany, 1941entire aluminum industry, D.G. Altenpohl’s volume (Ref 13) is • Casting, Vol 15, ASM Handbook, ASM International, 1988recommended. • S. Das, The Life Cycle Impacts of Aluminum Body-in-White Automotive Material, JOM, Aug 2000REFERENCES • J.R. Davis, Ed., ASM Specialty Handbook: Aluminum and Alu-1. Principles of Purchasing Castings, CD-ROM, American minum Alloys, ASM International, 1993 Foundry Society, 2002 • Design and Procurement of High-Strength Structural Alumi-2. U.S. Department of Commerce num Castings, American Foundrymen’s Society, 1995, 48 pages3. S. Das, The Life Cycle Impacts of Aluminum Body-in-White • J.D. Edwards, F.C. Frary, and Z. Jeffries, The Aluminum In- Automotive Material, JOM, Vol 52 (No. 8), Aug 2000, p 41–44 dustry, McGraw Hill, 19304. “Metalcasting Industry Technology Roadmap,” Cast Metal • Forgings and Castings, Vol 5, 8th ed., Metals Handbook, Ameri- Coalition, American Foundrymen’s Society, North American can Society for Metals, 1970 Die Casting Association, and Steel Founders’ Society of • M.B.W. Graham and B.H. Pruitt, R&D for Industry: A Century America, Jan 19985. “U.S. Energy Requirements for Aluminum Production,” The of Technical Innovation at Alcoa, Cambridge University Press, U.S. Dept. of Energy, Jan 2003 19906. D. Zalenas, Ed., Aluminum Casting Technology, 2nd ed., • J.E. Hatch, Ed., Aluminum: Properties and Physical Metal- American Foundrymen’s Society, 1993 lurgy, American Society for Metals, 19847. “NADCA Product Speciﬁcation Standards for Die Casting,” • J.G. Kaufman, Introduction to Aluminum Alloys and Tempers, 5th ed., North American Die Casting Association (NADCA), ASM International, 2000 2003 • Melting and Recycling of Aluminum Alloys, American Found-8. “Product Design for Die Casting in Recyclable Aluminum, rymen’s Society, 1997, 66 pages Magnesium, Zinc, and ZA Alloys,” Die Casting Development • The Physical Metallurgy of Aluminum Alloys, American Soci- Council, 19969. “The NFFS Guide to Aluminum Casting Design: Sand and ety for Metals, 1949 Permanent Mold,” Non-Ferrous Founders Society, 1994 • Properties and Selection: Nonferrous Alloys and Special-10. “Designations and Chemical Composition Limits for Alumi- Purpose Materials, Vol 2, ASM Handbook, ASM International, num Alloys in the Form of Castings and Ingot,” The Aluminum 1990 Association Alloy and Temper Registrations Records, The Alu- • E.L. Rooy, Scrap Recycling and Its Impact on the Metal Cast- minum Association, Jan, 1996 ings Industry, AFS Trans., l98511. “Aluminum Standards & Data (Standard and Metric Edi- • G.D. Smith, From Monopoly to Competition, Cambridge Uni- tions),” The Aluminum Association, published periodically versity Press, 198812. “Standards for Aluminum Sand and Permanent Mold Cast- • Solidiﬁcation Characteristics of Aluminum Alloys, Vol 2, ing,” The Aluminum Association, Dec 199213. D.G. Altenpohl, Aluminum: Technology, Applications and En- Foundry Alloys, American Foundrymen’s Society, 1990, 266 vironment, The Aluminum Association and TMS, 1999 pages • Solidiﬁcation Characteristics of Aluminum Alloys, Vol 3, Den-SELECTED REFERENCES drite Coherency, American Foundrymen’s Society, 1996, 258 pages• Aluminum and Aluminum Alloys, The Pittsburgh Reduction • K.R. Van Horn, Ed., Aluminum, Vol 1–3, American Society for Company, 1897 Metals, 1967
8 / Aluminum Alloy Castings: Properties, Processes, and Applications• Major alloying elements deﬁne the ranges of elements that Variations in the composition limits that are too small to require control castability and property development. a change in numeric designation are indicated by a preceding letter• Minor alloying elements control solidiﬁcation behavior, modify (A, B, C, etc). The ﬁrst version of an alloy, say 356.0, contains no eutectic structure, reﬁne primary phases, reﬁne grain size and letter preﬁx; the ﬁrst variation has an A, e.g., A356.0, the second form, promote or suppress phase formation, and reduce oxi- a B, for example, B356.0, and so forth. dation. The ﬁrst digit deﬁnes the major alloying constituent or constitu-• Impurity elements inﬂuence castability and the form of in- ents, with the following categories being deﬁned: soluble phases that at times limit or promote desired properties. • lxx.x, pure aluminum (99.00% or greater)Preferred major, minor, and impurity element concentrations and • 2xx.x, aluminum-copper alloysrelationships may not be deﬁned by alloy speciﬁcations. Optimal • 3xx.x, aluminum-silicon ϩ copper and/or magnesiumresults are not implied by nominal chemistries. The addition of • 4xx.x, aluminum-siliconstructure-controlling elements or combinations of elements can be • 5xx.x, aluminum-magnesiumcontained within chemistry limits when not otherwise speciﬁed • 7xx.x, aluminum-zincunder “Other Elements Each.” • 8xx.x, aluminum-tin Stoichiometric ratios for favored phase formation can be speci- • 9xx.x, aluminum ϩ other elementsﬁed, but also may not be controlled or deﬁned. • 6xx.x, unused series Concentration limits allow biasing of composition for castabilityand property development. For maximum strength, the concen- In designations of the 1xx.x type, the second and third digits in-tration of elements that form hardening phases can be maximized. dicate minimum aluminum content (99.00% or greater); these dig-Improved ductility results from ﬁner structures, restricting in- its are the same as the two to the right of the decimal point in thesoluble-element concentrations, and by controlling the concentra- minimum aluminum percentage expressed to the nearest 0.01%.tions of impurities in ratios that favor the formation of the least For example, alloy 170.0 contains a minimum of 99.70% Al.detrimental intermetallic constituents. Composition biasing can be In 2xx.x through 8xx.x designations for aluminum alloys, thespeciﬁed in ingot procurement or can result from alloying adjust- second and third digits have no numerical signiﬁcance, but onlyments in the foundry. arbitrarily identify individual alloys in the group. In all casting alloy designations, the fourth digit, that to the right of the decimal point, indicates product form:2.3 Alloy Designations • 0 denotes castings • 1 denotes standard ingot Designation systems and alloy nomenclature for aluminum cast- • 2 denotes ingot having composition ranges narrower than buting alloys are not internationally standardized. Many nations have within those of standard ingotdeveloped and published their own standards. Individual ﬁrmshave also promoted alloys by proprietary designations. In NorthAmerica, the most commonly used system is that developed and Designations in the form xxx.1 and xxx.2 include the compositionmaintained by the Aluminum Association. General procurement of speciﬁc alloys in remelt ingot form suitable for foundry use.speciﬁcations issued through government agencies and technical Designations in the form xxx.0 in all cases deﬁne compositionassociations and societies typically reference this nomenclature. limits applicable to castings. Further variations in speciﬁed com- positions are denoted by preﬁx letters used primarily to deﬁne differences in impurity limits. Accordingly, one of the most com-2.3.1 The Aluminum Association (AA) Casting Alloy mon gravity cast alloys, 356, has variations A356, B356, and C356; Designation System each of these alloys has identical major alloy contents, but has The most widely used casting alloy designation system in the decreasing speciﬁcation limits applicable to impurities, especiallyUnited States is the Aluminum Association (AA) alloy and temper iron content.systems (Ref 1), which are described below. Regrettably, the AA Alloying-element and impurity limits for ingot are usually thesystem is not universally used, and some of its earlier modiﬁcations same as those for castings of the same alloy. When the ingot isare still widely quoted. Therefore, subsequent sections discuss the remelted, iron and silicon contents tend to increase and magnesiumearlier variations as well as other rather widely used designations. content decreases. For these reasons, ingot chemistry for some In the AA alloy designation, there are four numeric digits, with alloys may be somewhat different from those speciﬁed for castings.a period between the third and fourth. The meanings of the four Despite the broad acceptance of the AA casting alloy designationdigits are: system, including recognition by the American National Standards Institute (ANSI), it remains relatively common to see the alloys• First digit: Principal alloying constituent(s) listed with only the ﬁrst three digits of the alloy designation, for• Second and third digits: Speciﬁc alloy designation (number has example, for 356.0, one may see simply 356 (see Section 2.3.3 in no signiﬁcance but is unique) this chapter). Technically, this is obsolete usage of the designation• Fourth digit: Casting (0) or ingot (1, 2) designation system, and for cast components the “.0” should always be utilized.
Chapter 2: Aluminum Casting Alloys / 9 The nominal compositions and composition limits of aluminum formal basis. They cause confusion because there is no obvious linkalloys in commercial use today are presented in Table 2.1. to the current system if one does not have a conversion guide such as Table 18.104.22.168.2 Aluminum Association Casting Temper The other fairly often seen variation is the result of the signiﬁcant Designation System revision of the Aluminum Association system in around 1990, The Aluminum Association Casting Temper Designation System when the guidelines for registering the alloys including copper and(Ref 1) uses letters and numbers to indicate the major types of magnesium were changed. The result was that some alloys shiftedthermal treatments applicable to engineered castings: classiﬁcation; for example, alloy 195.0 became 295.0 and alloy 214.0 became 514.0.• F, as-cast• O, annealed 2.3.4 The UNS Alloy Designation System• T4, solution treated and aged Another rather widely known alloy classiﬁcation system is the• T5, precipitation hardened Uniﬁed Numbering System (UNS) (Ref 2). The UNS system has• T6, solution heat treated, quenched, and precipitation hardened the advantage of covering all metallic alloy systems.• T7, solution heat treated, quenched, and overaged For aluminum alloys, as illustrated in Table 2.2, this system is essentially an adaptation of the Aluminum Association alloy des- Temper designation is presented immediately following the alloy ignation system to ﬁt the UNS format. UNS numbers are obtaineddesignation. Thus, for a 356.0 alloy casting that has been solution by taking the three digits to the left of the decimal point in theheat treated, quenched, and artiﬁcially aged, the full alloy and Aluminum Association system and adding A9 (meaning aluminumtemper designation would be shown as 356.0-T6. Examples of alloys) and a digit reﬂecting the letter preﬁx to the alloy desig-registered temper variations are A357.0-T61, 242.0-T571, and nation. For alloys with no letter preﬁx, the next numeric digit after355.0-T71. A9 is a 0; for those with A, the next digit is 1, for B, it is 2, and Other variations of temper designations are permitted by the so forth.Aluminum Association Temper Designation System (Ref 1), the Thus, in the UNS system, 356.0 becomes A90356, A356.0 be-most common being the use of “P” added to a standard temper comes A91356, C356.0 becomes A93356; and so forth.designation (e.g., T6P) indicating a producer variation of the stan- The UNS system is not as widely used for aluminum alloys asdard processing treatment. There is further discussion of temper for certain other classes of alloys. An example would be copperdesignations in Chapter 7, “Heat Treatment of Aluminum Cast- alloys, for which the UNS designations have been selected as theings.” U.S. standards.2.3.3 Evolution of Designation System; 2.3.5 International Casting Alloy Designations Cross-Reference to Older Designations Unlike the case for wrought aluminum alloys, there is no inter- As noted previously, over the years there have been several national accord on casting alloy designations, and other systems areevolutionary steps in the development of the Aluminum Associa- rather universally used overseas (Ref 3). Most systems employtion casting alloy designation system, with the result that it is not some system based on identifying the major alloying elements, butuncommon to ﬁnd variations of the current designations appearing regrettably there are many variations of these.on drawings and in publications from not too many years ago, and One of the mostly widely used international systems is the Eu-in some cases even in current publications. To assist in dealing with ronorm designation, and so, where applicable, designations of thatsuch variations, Table 2.2 illustrates a number of the variations in type have been included in Table 2.2. There are no comparablecasting alloy designations over the past 50 years. Euronorm designations for about half of the alloys registered in the The overall most common variation is clearly the omission of the United States, nor is there any simple guide to generate them.decimal point and the fourth digit, always a .0 for a foundry prod-uct. While inconsistent with current Aluminum Association stan-dards, this variation is not usually a problem resulting in confusion, 2.3.6 Nomenclature System for Aluminumas for example it is relatively clear that an alloy designated 354 may Metal-Matrix Compositessafely be assumed to be 354.0 by today’s standard system. Aluminum casting alloys are now regularly used as the matrix While the most common variation is the omission of the decimal material in metal-matrix composites (MMC). The Aluminum As-point and the fourth digit in the designation, there are two other sociation, Inc, and ANSI H35.5 (Ref 4) have published a standardtypes of variations reﬂected in Table 2.2 that are also seen fre- nomenclature system for such composites that builds on the stan-quently and can be more confusing. One variation is simply a dard casting alloy designation system as outlined below. Althoughproprietary designation that has become rather widely known in the this standard nomenclature has been established, some MMC sup-past, for example, Hiduminium, Frontier 40E, Precedent 71, and pliers have preferred their own designations. One reason is thatAlmag 35. These designations originated before the alloy compo- matrix alloys may not coincide exactly with Aluminum Associationsitions were registered with the Aluminum Association and had no ranges.